LMucko/crystallography-open-database huggingface dataset:
Crystal chemistry and structural refinement of chromites from different chromitite layers and xenoliths of the Bushveld complex Sample: BV29A, UG2
Lenaz, D.; Braidotti, R.; Princivalle, F.; Garuti, G.; Zaccarini, F.; European Journal of Mineralogy 19 (2007) 599–609; doi:10.1127/0935-1221/2007/0019-1744

data_9010823
_publ_section_title
;
 Crystal chemistry and structural refinement of chromites from different
 chromitite layers and xenoliths of the Bushveld complex
 Sample: BV29A, UG2
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               609
_journal_paper_doi               10.1127/0935-1221/2007/0019-1744
_journal_volume                  19
_journal_year                    2007
_chemical_compound_source        'Bushveld complex, South Africa'
_chemical_formula_sum
'Al0.679 Cr1.082 Fe0.755 Mg0.439 Mn0.007 Ni0.004 O4 Ti0.024 V0.01'
_chemical_name_mineral           Chromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.2942
_cell_length_b                   8.2942
_cell_length_c                   8.2942
_cell_volume                     570.589
_database_code_amcsd             0007237
_exptl_crystal_density_diffrn    4.509
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum
'Al.679 Fe.755 Mg.439 Mn.007 Cr1.082 Ni.004 Ti.024 V.01 O4'
_cod_database_code               9010823
_cell_formula_units_Z 8
Crystal chemistry and structural refinement of chromites from different chromitite layers and xenoliths of the Bushveld complex Sample: BV32, UG2
Lenaz, D.; Braidotti, R.; Princivalle, F.; Garuti, G.; Zaccarini, F.; European Journal of Mineralogy 19 (2007) 599–609; doi:10.1127/0935-1221/2007/0019-1744

data_9010824
_publ_section_title
;
 Crystal chemistry and structural refinement of chromites from different
 chromitite layers and xenoliths of the Bushveld complex
 Sample: BV32, UG2
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               609
_journal_paper_doi               10.1127/0935-1221/2007/0019-1744
_journal_volume                  19
_journal_year                    2007
_chemical_compound_source        'Bushveld complex, South Africa'
_chemical_formula_sum
'Al0.679 Cr1.062 Fe0.754 Mg0.462 Mn0.007 Ni0.006 O4 Ti0.02 V0.01'
_chemical_name_mineral           Chromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.2944
_cell_length_b                   8.2944
_cell_length_c                   8.2944
_cell_volume                     570.630
_database_code_amcsd             0007238
_exptl_crystal_density_diffrn    4.495
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum
'Al.679 Fe.754 Mg.462 Mn.007 Cr1.062 Ni.006 Ti.02 V.01 O4'
_cod_database_code               9010824
_cell_formula_units_Z 8
Crystal chemistry and structural refinement of chromites from different chromitite layers and xenoliths of the Bushveld complex Sample: BV32A, UG2
Lenaz, D.; Braidotti, R.; Princivalle, F.; Garuti, G.; Zaccarini, F.; European Journal of Mineralogy 19 (2007) 599–609; doi:10.1127/0935-1221/2007/0019-1744

data_9010825
_publ_section_title
;
 Crystal chemistry and structural refinement of chromites from different
 chromitite layers and xenoliths of the Bushveld complex
 Sample: BV32A, UG2
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               609
_journal_paper_doi               10.1127/0935-1221/2007/0019-1744
_journal_volume                  19
_journal_year                    2007
_chemical_compound_source        'Bushveld complex, South Africa'
_chemical_formula_sum
'Al0.667 Cr1.07 Fe0.747 Mg0.468 Mn0.007 Ni0.006 O4 Ti0.022 V0.01 Zn0.003'
_chemical_name_mineral           Chromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.2950
_cell_length_b                   8.2950
_cell_length_c                   8.2950
_cell_volume                     570.754
_database_code_amcsd             0007239
_exptl_crystal_density_diffrn    4.497
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum
'Al.667 Fe.747 Mg.468 Mn.007 Zn.003 Cr1.07 Ni.006 Ti.022 V.01 O4'
_cod_database_code               9010825
_cell_formula_units_Z 8
Crystal chemistry and structural refinement of chromites from different chromitite layers and xenoliths of the Bushveld complex Sample: BV31, UG3
Lenaz, D.; Braidotti, R.; Princivalle, F.; Garuti, G.; Zaccarini, F.; European Journal of Mineralogy 19 (2007) 599–609; doi:10.1127/0935-1221/2007/0019-1744

data_9010826
_publ_section_title
;
 Crystal chemistry and structural refinement of chromites from different
 chromitite layers and xenoliths of the Bushveld complex
 Sample: BV31, UG3
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               609
_journal_paper_doi               10.1127/0935-1221/2007/0019-1744
_journal_volume                  19
_journal_year                    2007
_chemical_compound_source        'Bushveld complex, South Africa'
_chemical_formula_sum
'Al0.685 Cr1.068 Fe0.739 Mg0.464 Mn0.007 Ni0.008 O4 Ti0.018 V0.008 Zn0.003'
_chemical_name_mineral           Chromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.2902
_cell_length_b                   8.2902
_cell_length_c                   8.2902
_cell_volume                     569.764
_database_code_amcsd             0007240
_exptl_crystal_density_diffrn    4.497
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum
'Al.685 Fe.739 Mg.464 Mn.007 Zn.003 Cr1.068 Ni.008 Ti.018 V.008 O4'
_cod_database_code               9010826
_cell_formula_units_Z 8
Crystal chemistry and structural refinement of chromites from different chromitite layers and xenoliths of the Bushveld complex Sample: BV31A, UG3
Lenaz, D.; Braidotti, R.; Princivalle, F.; Garuti, G.; Zaccarini, F.; European Journal of Mineralogy 19 (2007) 599–609; doi:10.1127/0935-1221/2007/0019-1744

data_9010827
_publ_section_title
;
 Crystal chemistry and structural refinement of chromites from different
 chromitite layers and xenoliths of the Bushveld complex
 Sample: BV31A, UG3
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               609
_journal_paper_doi               10.1127/0935-1221/2007/0019-1744
_journal_volume                  19
_journal_year                    2007
_chemical_compound_source        'Bushveld complex, South Africa'
_chemical_formula_sum
'Al0.698 Cr1.064 Fe0.727 Mg0.469 Mn0.007 Ni0.006 O4 Ti0.018 V0.008 Zn0.003'
_chemical_name_mineral           Chromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.2900
_cell_length_b                   8.2900
_cell_length_c                   8.2900
_cell_volume                     569.723
_database_code_amcsd             0007241
_exptl_crystal_density_diffrn    4.485
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum
'Al.698 Fe.727 Mg.469 Mn.007 Zn.003 Cr1.064 Ni.006 Ti.018 V.008 O4'
_cod_database_code               9010827
_cell_formula_units_Z 8
Crystal chemistry and structural refinement of chromites from different chromitite layers and xenoliths of the Bushveld complex Sample: BV30, UG3B
Lenaz, D.; Braidotti, R.; Princivalle, F.; Garuti, G.; Zaccarini, F.; European Journal of Mineralogy 19 (2007) 599–609; doi:10.1127/0935-1221/2007/0019-1744

data_9010828
_publ_section_title
;
 Crystal chemistry and structural refinement of chromites from different
 chromitite layers and xenoliths of the Bushveld complex
 Sample: BV30, UG3B
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               609
_journal_paper_doi               10.1127/0935-1221/2007/0019-1744
_journal_volume                  19
_journal_year                    2007
_chemical_compound_source        'Bushveld complex, South Africa'
_chemical_formula_sum
'Al0.62 Cr1.072 Fe0.842 Mg0.408 Mn0.009 Ni0.006 O4 Ti0.032 V0.01 Zn0.001'
_chemical_name_mineral           Chromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.2994
_cell_length_b                   8.2994
_cell_length_c                   8.2994
_cell_volume                     571.663
_database_code_amcsd             0007242
_exptl_crystal_density_diffrn    4.563
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum
'Fe.842 Mg.408 Mn.009 Zn.001 Al.62 Cr1.072 Ni.006 Ti.032 V.01 O4'
_cod_database_code               9010828
_cell_formula_units_Z 8
Crystal chemistry and structural refinement of chromites from different chromitite layers and xenoliths of the Bushveld complex Sample: BV30A, UG3B
Lenaz, D.; Braidotti, R.; Princivalle, F.; Garuti, G.; Zaccarini, F.; European Journal of Mineralogy 19 (2007) 599–609; doi:10.1127/0935-1221/2007/0019-1744

data_9010829
_publ_section_title
;
 Crystal chemistry and structural refinement of chromites from different
 chromitite layers and xenoliths of the Bushveld complex
 Sample: BV30A, UG3B
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               609
_journal_paper_doi               10.1127/0935-1221/2007/0019-1744
_journal_volume                  19
_journal_year                    2007
_chemical_compound_source        'Bushveld complex, South Africa'
_chemical_formula_sum
'Al0.541 Cr1.118 Fe0.873 Mg0.406 Mn0.009 Ni0.006 O4 Ti0.034 V0.01 Zn0.003'
_chemical_name_mineral           Chromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3013
_cell_length_b                   8.3013
_cell_length_c                   8.3013
_cell_volume                     572.056
_database_code_amcsd             0007243
_exptl_crystal_density_diffrn    4.610
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum
'Al.541 Fe.873 Mg.406 Mn.009 Zn.003 Cr1.118 Ni.006 Ti.034 V.01 O4'
_cod_database_code               9010829
_cell_formula_units_Z 8
Crystal chemistry and structural refinement of chromites from different chromitite layers and xenoliths of the Bushveld complex Sample: MER, MR
Lenaz, D.; Braidotti, R.; Princivalle, F.; Garuti, G.; Zaccarini, F.; European Journal of Mineralogy 19 (2007) 599–609; doi:10.1127/0935-1221/2007/0019-1744

data_9010830
_publ_section_title
;
 Crystal chemistry and structural refinement of chromites from different
 chromitite layers and xenoliths of the Bushveld complex
 Sample: MER, MR
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               609
_journal_paper_doi               10.1127/0935-1221/2007/0019-1744
_journal_volume                  19
_journal_year                    2007
_chemical_compound_source        'Bushveld complex, South Africa'
_chemical_formula_sum
'Al0.582 Cr1.168 Fe0.752 Mg0.453 Mn0.008 Ni0.006 O4 Ti0.022 V0.008 Zn0.001'
_chemical_name_mineral           Chromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.2929
_cell_length_b                   8.2929
_cell_length_c                   8.2929
_cell_volume                     570.321
_database_code_amcsd             0007244
_exptl_crystal_density_diffrn    4.560
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum
'Fe.752 Mg.453 Mn.008 Zn.001 Al.582 Cr1.168 Ni.006 Ti.022 V.008 O4'
_cod_database_code               9010830
_cell_formula_units_Z 8
Crystal chemistry and structural refinement of chromites from different chromitite layers and xenoliths of the Bushveld complex Sample: MER-A, MR
Lenaz, D.; Braidotti, R.; Princivalle, F.; Garuti, G.; Zaccarini, F.; European Journal of Mineralogy 19 (2007) 599–609; doi:10.1127/0935-1221/2007/0019-1744

data_9010831
_publ_section_title
;
 Crystal chemistry and structural refinement of chromites from different
 chromitite layers and xenoliths of the Bushveld complex
 Sample: MER-A, MR
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               609
_journal_paper_doi               10.1127/0935-1221/2007/0019-1744
_journal_volume                  19
_journal_year                    2007
_chemical_compound_source        'Bushveld complex, South Africa'
_chemical_formula_sum
'Al0.618 Cr1.126 Fe0.745 Mg0.467 Mn0.008 Ni0.006 O4 Ti0.022 V0.008'
_chemical_name_mineral           Chromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.2963
_cell_length_b                   8.2963
_cell_length_c                   8.2963
_cell_volume                     571.023
_database_code_amcsd             0007245
_exptl_crystal_density_diffrn    4.523
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum
'Fe.745 Mg.467 Mn.008 Al.618 Cr1.126 Ni.006 Ti.022 V.008 O4'
_cod_database_code               9010831
_cell_formula_units_Z 8
Crystal chemistry of synthetic Co- and Ni-analogues of natrochalcite - the shortest known hydrogen bonds among mineral-type compounds Part I: single-crystal X-ray structures Sample: T = 293 K
Krickl, R.; Wildner, M.; European Journal of Mineralogy 19 (2007) 805–816; doi:10.1127/0935-1221/2007/0019-1770

data_9010832
_publ_section_title
;
 Crystal chemistry of synthetic Co- and Ni-analogues of natrochalcite - the
 shortest known hydrogen bonds among mineral-type compounds
 Part I: single-crystal X-ray structures
 Sample: T = 293 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              805
_journal_page_last               816
_journal_paper_doi               10.1127/0935-1221/2007/0019-1770
_journal_volume                  19
_journal_year                    2007
_chemical_formula_sum            'Co2 H3 Na O10 S2'
_chemical_name_mineral           NaCoS
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 115.40
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.677
_cell_length_b                   6.317
_cell_length_c                   7.396
_cell_volume                     366.207
_database_code_amcsd             0007246
_diffrn_ambient_temperature      293
_exptl_crystal_density_diffrn    3.337
_cod_original_formula_sum        'Na Co2 S2 O10 H3'
_cod_database_code               9010832
_amcsd_formula_title             NaCo2S2O10H3
Crystal chemistry of synthetic Co- and Ni-analogues of natrochalcite - the shortest known hydrogen bonds among mineral-type compounds Part I: single-crystal X-ray structures Sample: T = 105 K
Krickl, R.; Wildner, M.; European Journal of Mineralogy 19 (2007) 805–816; doi:10.1127/0935-1221/2007/0019-1770

data_9010833
_publ_section_title
;
 Crystal chemistry of synthetic Co- and Ni-analogues of natrochalcite - the
 shortest known hydrogen bonds among mineral-type compounds
 Part I: single-crystal X-ray structures
 Sample: T = 105 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              805
_journal_page_last               816
_journal_paper_doi               10.1127/0935-1221/2007/0019-1770
_journal_volume                  19
_journal_year                    2007
_chemical_formula_sum            'Co2 H3 Na O10 S2'
_chemical_name_mineral           NaCoS
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 115.41
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.659
_cell_length_b                   6.281
_cell_length_c                   7.368
_cell_volume                     361.959
_database_code_amcsd             0007247
_diffrn_ambient_temperature      105
_exptl_crystal_density_diffrn    3.377
_cod_original_formula_sum        'Na Co2 S2 O10 H3'
_cod_database_code               9010833
_amcsd_formula_title             NaCo2S2O10H3
Crystal chemistry of synthetic Co- and Ni-analogues of natrochalcite - the shortest known hydrogen bonds among mineral-type compounds Part I: single-crystal X-ray structures Sample: T = 293 K
Krickl, R.; Wildner, M.; European Journal of Mineralogy 19 (2007) 805–816; doi:10.1127/0935-1221/2007/0019-1770

data_9010834
_publ_section_title
;
 Crystal chemistry of synthetic Co- and Ni-analogues of natrochalcite - the
 shortest known hydrogen bonds among mineral-type compounds
 Part I: single-crystal X-ray structures
 Sample: T = 293 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              805
_journal_page_last               816
_journal_paper_doi               10.1127/0935-1221/2007/0019-1770
_journal_volume                  19
_journal_year                    2007
_chemical_formula_sum            'H3 Na Ni2 O10 S2'
_chemical_name_mineral           NaNiS
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 114.78
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.605
_cell_length_b                   6.185
_cell_length_c                   7.336
_cell_volume                     354.486
_database_code_amcsd             0007248
_diffrn_ambient_temperature      293
_exptl_crystal_density_diffrn    3.443
_cod_original_formula_sum        'Na Ni2 S2 O10 H3'
_cod_database_code               9010834
_amcsd_formula_title             NaNi2S2O10H3
Crystal chemistry of synthetic Co- and Ni-analogues of natrochalcite - the shortest known hydrogen bonds among mineral-type compounds Part I: single-crystal X-ray structures Sample: T = 105 K
Krickl, R.; Wildner, M.; European Journal of Mineralogy 19 (2007) 805–816; doi:10.1127/0935-1221/2007/0019-1770

data_9010835
_publ_section_title
;
 Crystal chemistry of synthetic Co- and Ni-analogues of natrochalcite - the
 shortest known hydrogen bonds among mineral-type compounds
 Part I: single-crystal X-ray structures
 Sample: T = 105 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              805
_journal_page_last               816
_journal_paper_doi               10.1127/0935-1221/2007/0019-1770
_journal_volume                  19
_journal_year                    2007
_chemical_formula_sum            'H3 Na Ni2 O10 S2'
_chemical_name_mineral           NaNiS
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 114.81
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.595
_cell_length_b                   6.172
_cell_length_c                   7.319
_cell_volume                     352.426
_database_code_amcsd             0007249
_diffrn_ambient_temperature      105
_exptl_crystal_density_diffrn    3.463
_cod_original_formula_sum        'Na Ni2 S2 O10 H3'
_cod_database_code               9010835
_amcsd_formula_title             NaNi2S2O10H3
Crystal chemistry of synthetic Co- and Ni-analogues of natrochalcite - the shortest known hydrogen bonds among mineral-type compounds Part I: single-crystal X-ray structures Sample: T = 293 K
Krickl, R.; Wildner, M.; European Journal of Mineralogy 19 (2007) 805–816; doi:10.1127/0935-1221/2007/0019-1770

data_9010836
_publ_section_title
;
 Crystal chemistry of synthetic Co- and Ni-analogues of natrochalcite - the
 shortest known hydrogen bonds among mineral-type compounds
 Part I: single-crystal X-ray structures
 Sample: T = 293 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              805
_journal_page_last               816
_journal_paper_doi               10.1127/0935-1221/2007/0019-1770
_journal_volume                  19
_journal_year                    2007
_chemical_formula_sum            'Co2 H3 Na O10 Se2'
_chemical_name_mineral           NaCoSe
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 115.09
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.939
_cell_length_b                   6.382
_cell_length_c                   7.554
_cell_volume                     390.283
_database_code_amcsd             0007250
_diffrn_ambient_temperature      293
_exptl_crystal_density_diffrn    3.930
_cod_original_formula_sum        'Na Co2 Se2 O10 H3'
_cod_database_code               9010836
_amcsd_formula_title             NaCo2Se2O10H3